Biological Performances of Plasmonic Biohybrids Based on Phyto-Silver/Silver Chloride Nanoparticles

Silver/silver chloride nanoparticles (Ag/AgClNPs), with a mean size of 48.2 ± 9.5 nm and a zeta potential value of −31.1 ± 1.9 mV, obtained by the Green Chemistry approach from a mixture of nettle and grape extracts, were used as “building blocks” for the “green” development of plasmonic biohybrids containing biomimetic membranes and chitosan. The mechanism of biohybrid formation was elucidated by optical analyses (UV–vis absorption and emission fluorescence, FTIR, XRD, and SAXS) and microscopic techniques (AFM and SEM). The aforementioned novel materials showed a free radical scavenging capacity of 75% and excellent antimicrobial properties against Escherichia coli (IGZ = 45 mm) and Staphylococcus aureus (IGZ = 35 mm). The antiproliferative activity of biohybrids was highlighted by a therapeutic index value of 1.30 for HT-29 cancer cells and 1.77 for HepG2 cancer cells. At concentrations below 102.2 µM, these materials are not hemolytic, so they will not be harmful when found in the bloodstream. In conclusion, hybrid systems based on phyto-Ag/AgClNPs, artificial cell membranes, and chitosan can be considered potential adjuvants in liver and colorectal cancer treatment.


Introduction
Nowadays, the use of natural resources and, in particular, plants has experienced a great importance, thanks to the impressive number of bioactive ingredients with a strong beneficial impact on human health. The intensive development of new hybrid lipidnanoparticle complexes, including inorganic nanoparticles (NPs), lipid assemblies, and lipid-polymer complexes, is caused by numerous potential biomedical applications [1,2]. Soy lecithin liposomes represent a promising drug delivery system, especially in the from Merck (Darmstadt, Germany). Standard hemoglobin, soybean lecithin, NaCl, Drabkin reagent, ethidium homodimer-1 (EthD-1), and acridine orange (AO) were purchased from Sigma-Aldrich (Darmstadt, Germany). The yeast extract was supplied from BioLife, and the agar was obtained from Fluka (Switzerland). Chlorophyll a was extracted in our laboratory from fresh spinach leaves according to the method of Strain and Svec [23]. The nettle leaves and the grapes were acquired from a local market.
Bacteria culture test. Antimicrobial activity of the samples was tested against pathogenic Gram (-) bacteria Escherichia coli ATCC 8738 and Gram (+) bacteria Staphylococcus aureus ATTC 25923. These bacterial cultures were maintained at 4 • C. All chemicals used for antibacterial investigations were purchased from VWR (Darmstadt, Germany).
Cell culture and reagents. Three different cell lines were used for the in vitro studies. Human fibroblast BJ cells (ATCC CRL-2522, Manassas, VA, USA) and human colorectal adenocarcinoma HT-29 cells (ATCC, Manassas, VA, USA) were grown in Minimal Essential Medium (MEM) supplemented with 2 mM L-Glutamine, 10% fetal calf serum (FCS), 100 units/mL of penicillin, and 100 µg/mL of streptomycin at 37 • C in a humidified incubator under an atmosphere containing 5% CO 2 . Human hepatocarcinoma HepG2 cells (ATCC, Manassas, VA, USA) were grown in DMEM supplemented with similar reagents. All cell cultivation media and reagents were purchased from Biochrom AG (Berlin, Germany). Drabkin reagent and standard hemoglobin were purchased from Sigma-Aldrich (Darmstadt, Germany).

Preparation of Nanosilver-Based Biohybrids 2.2.1. Phytogeneration of Silver/Silver Chloride Nanoparticles
Two types of aqueous extracts of nettle leaves and grapes were prepared as described in [22]. A mixture of (0.24 mL of nettle extract + 0.06 mL of grape extract) was added to a volume of 30 mL of 1 mM AgNO 3 aqueous solution, under continuous magnetic stirring, and then placed at room temperature for one day. This suspension was diluted 1.62 times with phosphate-buffered saline (PBS, KH 2 PO 4 /Na 2 HPO 4 /NaCl, pH 7.4) and furthermore subjected to an ultrasound treatment in an ultrasonic bath (BRANSON 1210, Marshall Scientific, Hampton, NH, USA) for 30 min. The resulting Ag/AgClNPs were diluted in the biodispersant PBS to a final silver content of 0.61 mM.

Preparation of Artificial Cell Membranes
Artificial cell membranes labeled with Chla were obtained by the hydration of soybean lecithin thin as previously described [24]. The resulting liposome suspensions were divided into two parts: without and with chitosan. An acidic solution (0.4% acetic acid v/v in distilled water) of 1% (w/v) chitosan (CTS) was added to a liposomal suspension, to a final CTS concentration of 0.01% (w/v); this mixture was then strongly stirred for 15 min (200 rpm, VIBRAX stirrer, Milian, OH, USA). These two types of biological entities were further diluted in PBS to a final lipid concentration of 0.34 mg/mL.

Bottom-up "Green" Design of Plasmonic Biohybrids
Three types of hybrid silver-based systems were prepared based on suspensions of Ag/AgClNPs and liposomes, with and without chitosan solution, according to Table 1 (see Samples P4-P6) by using strong stirring (VIBRAX stirrer, Milian, OH USA 200 rpm) for 15 min and ultrasound treatment in an ultrasonic bath (BRANSON 1210, Marshall Scientific, Hampton, NH, USA) for 30 min.
All these biohybrids were diluted in PBS to a final lipid concentration of 0.34 mg/mL and with a final silver content of 0.61 mM. Figure 1 shows a diagram representing the "green" development of biohybrids generated from the aqueous extract of a mixture of nettle and grape extracts.  Ag/AgClNPs-Liposomes-CTS (Biohybrid III) 0.34 0.61 0.01 Figure 1 shows a diagram representing the "green" development of biohybrids generated from the aqueous extract of a mixture of nettle and grape extracts.

Spectral and Morphological Characterization
The absorption spectra of the samples were recorded (at the resolution of 1 nm) from 200 to 800 nm on a double-beam Jasco V-670 UV-vis-NIR spectrophotometer (Jasco, Tokyo, Japan).
The fluorescence emission spectra of chlorophyll-a-based samples were collected using a LS55 Perkin Elmer fluorescence spectrometer (Waltham, MA, USA) in the wavelength range of 600-800 nm by illuminating the samples with a 430 nm excitation light.
Fourier-transform infrared (FTIR) spectra of initial components AgNPs, liposomes, and biohybrid complexes were recorded on an Excalibur FTS-3000 FTIR spectrometer (Bio-Rad, Munich, Germany), in the wavenumber range of 4000-500 cm −1 . Each spectrum was averaged over 128 scans, and the spectral resolution was 0.4 cm −1 at a constant temperature of 40 ± 1 °C. The samples were thin films, placed between two ZnSe window discs. During the recorded spectra, the spectrometer was purged with dry nitrogen. For all obtained spectra, the baseline correction and normalization were applied.
For atomic force microscopy (AFM) experiments, the sample solutions (50 µL aliquots) were deposited onto freshly cleaved 15 mm × 15 mm mica squares, left to adsorb for 3 min, and rinsed with Millipore water added dropwise to remove redundant samples. The surface was air dried (3 h) in a dust-free enclosure at room temperature, then imaged using AFM. Atomic force microscopy NTEGRA PRIMA was provided by NT-MDT Spectrum Instruments (Zelenograd, Russia). AFM images were recorded in tapping mode with commercial NSG01 tips of a 10 nm curvature radius (NT-MDT Spectrum Instruments, Zelenograd, Russia) at room temperature. Images were taken continuously at a scan rate of 0.3−0.5 Hz. Both the height image and the phase image were  The absorption spectra of the samples were recorded (at the resolution of 1 nm) from 200 to 800 nm on a double-beam Jasco V-670 UV-vis-NIR spectrophotometer (Jasco, Tokyo, Japan).
The fluorescence emission spectra of chlorophyll-a-based samples were collected using a LS55 Perkin Elmer fluorescence spectrometer (Waltham, MA, USA) in the wavelength range of 600-800 nm by illuminating the samples with a 430 nm excitation light.
Fourier-transform infrared (FTIR) spectra of initial components AgNPs, liposomes, and biohybrid complexes were recorded on an Excalibur FTS-3000 FTIR spectrometer (Bio-Rad, Munich, Germany), in the wavenumber range of 4000-500 cm −1 . Each spectrum was averaged over 128 scans, and the spectral resolution was 0.4 cm −1 at a constant temperature of 40 ± 1 • C. The samples were thin films, placed between two ZnSe window discs. During the recorded spectra, the spectrometer was purged with dry nitrogen. For all obtained spectra, the baseline correction and normalization were applied.
For atomic force microscopy (AFM) experiments, the sample solutions (50 µL aliquots) were deposited onto freshly cleaved 15 mm × 15 mm mica squares, left to adsorb for 3 min, and rinsed with Millipore water added dropwise to remove redundant samples. The surface was air dried (3 h) in a dust-free enclosure at room temperature, then imaged using AFM. Atomic force microscopy NTEGRA PRIMA was provided by NT-MDT Spectrum Instruments (Zelenograd, Russia). AFM images were recorded in tapping mode with commercial NSG01 tips of a 10 nm curvature radius (NT-MDT Spectrum Instruments, Zelenograd, Russia) at room temperature. Images were taken continuously at a scan rate of 0.3−0.5 Hz. Both the height image and the phase image were recorded. The images were flattened using the NT-MDT Spectrum Instruments Image Analysis P9 software.
The surface morphology of the samples presented in this paper was analyzed using a scanning electron microscope (SEM), a FEI Inspect Model S50 apparatus (Hillsboro, OR, USA). The apparatus is equipped with a secondary electrons (SE) detector. The SEM images were obtained at a 10 mm working distance, a 10 kV acceleration voltage, and for 50 up to 50,000× magnifications. Before SEM investigations, all the samples were coated with a thin Au layer (~10 nm). The Au layer was obtained using a sputtering Cressington 108 auto sputter coater apparatus (Cressington Scientific Instruments UK, Watford, England (UK)), equipped with a Cressington MTM-20 thickness controller. The ImageJ program was used to estimate the size of the developed materials from the magnified SEM images.
The hydrodynamic diameters (Zav) of samples were measured by the dynamic light scattering (DLS) technique (Zetasizer Nano ZS, Malvern Instruments Ltd., Worcestershire, U.K.), at a scattering angle of 90 • by the Stokes-Einstein equation. The mean values were calculated from three individual experiments, so the average values (±standard deviation, SD) were further reported. The polydispersity indexes (PdI-the indicator of the width of the particle size distribution) were also determined from 3 individual measurements using intensity distribution.
Zeta potential (ξ) measurements were carried out at 25 • C in triplicate, and the mean values were reported on Malvern Zetasizer Nano ZS (Malvern Instruments Inc., Worcestershire, UK) by measuring, in an electric field, the electrophoretic mobility of the prepared samples.
The crystallographic structure and phase composition of the sample series P3-P6 containing Ag/AgClNPs were examined by X-ray diffraction (XRD) by using an EMPYREAN diffractometer (PANalytical, Almelo, The Netherlands) with Cu-Kα incident radiation. Samples P3-P6 were extracted from the PBS solution by centrifuging (15,000× g, 30 min) at 4 • C. The separated upper layer (supernatant) was removed. The liquid sediment was placed on quartz glass (2.5 cm × 2.5 cm) and was evaporated in a vacuum chamber for 12 h at room temperature. The XRD spectra were measured with an exposition time of 12 h for each sample. The average sizes of nanoparticles for each phase were estimated using the Scherrer equation: where D is the average crystallite size, K is a dimensionless shape factor close to unity, λ is the X-ray wavelength, θ is the Bragg angle, and β is the peak width at half the maximum intensity (FWHM) after subtracting the instrumental line broadening. SAXS experiments were performed using a pinhole camera (MolMet, Rigaku, Japan, modified by SAXSLAB/Xenocs) attached to a microfocused X-ray beam generator (Rigaku MicroMax 003) operating at 50 kV and 0.6 mA (30 W). The camera was equipped with a vacuum version of the Pilatus 300 K detector. Calibration of primary beam position and sample-to-detector distances was performed using a AgBehenate sample. For the measurements, samples were sealed into borosilicate capillaries. Two experimental setups were used to cover the q range of 0.005-0.5 Å −1 . The scattering vector, q, is defined as q = (4π/λ)sin(Θ), where λ is the wavelength and 2Θ is the scattering angle. Homemade software based on the PyFAI Python library [25] was used for data reduction.

In Vitro Antioxidant Activity
The chemiluminescence (CL) technique (Turner Design TD 20/20 USA Chemiluminometer) was used to evaluate the antioxidant properties of the samples by using a free radical generator system based on 10 where I 0 and I are the maximum CL intensities at t = 5 s for the control (i.e., the reaction mixture without the sample) and for each sample, respectively [26].

Antibacterial Activity
Bacteria stock cultures (Staphylococcus aureus and Escherichia coli) were subcultured onto Luria Bertani Agar acc. Miller (LBA) plates at 37 • C. To evaluate the antibacterial properties of the tested samples, the antibacterial activity was determined by the agar well diffusion method as previously described in [27]. Briefly, the LBA surface was inoculated by spreading a volume of the bacteria inoculum. Using a sterile Durham tube 6 mm in diameter, the wells were made and inoculated with 50 µL of each sample; then, the Luria Bertani Agar plates were incubated at 37 • C for 24 h. The antimicrobial agent diffused into the LBA and inhibited the growth of the test bacteria, and then the diameters of the inhibition growth zones (IGZs) were measured.

Cell Viability
The biocompatibility of the biohybrids was evaluated using MTT (3-(4,5-dimethylthiazol-2-yl)-2,5-diphenyltetrazolium bromide) tetrazolium reduction assay as follows. Cells (BJ, HT-29, and HepG2) were seeded in 96-well plates and cultured for 24 h in medium. The next day, the medium was changed, and different concentrations of biohybrids were added for 24 h. Cells grown only in medium were used as negative control. Following incubation, the medium was changed, and 1 mg/mL of MTT solution was added to each well and incubated for an additional 4 h at 37 • C. Finally, the medium was collected, and DMSO was used to dissolve the insoluble formazan product. The absorbance of the samples was recorded at 570 nm using a Mithras 940 plate reader (Berthold, Germany). The data were corrected for the background, and the percentage of viable cells was obtained using the following equation: The NP concentration that reduced the viability of the cells by half (IC 50 ) was obtained by fitting the data with a logistical sigmoidal equation using the software Origin 8.1 (Microcal Inc., Northampton, MA, USA.). The therapeutic index (TI) was calculated as the ratio of the dose that produces toxicity to the dose needed to produce the desired therapeutic response [28].

Evaluation of Cellular Morphology
Cells were grown on coverslips and treated for 24 h with two different concentrations for the biohybrids. Afterwards, the cells were washed with PBS, fixed for 15 min with 3.7% formaldehyde dissolved in PBS, and washed again with PBS buffer. Sequentially, cells were stained with 20 µg/mL AO solution for 15 min, then immediately washed with PBS, followed imaging using an Andor DSD2 Confocal Unit (Andor, Belfast, Northern Ireland), mounted on an Olympus BX-51 epifluorescence microscope (Olympus, Hamburg, Germany), equipped with a 40× objective and an appropriate filter cube (excitation filter, 466/40 nm; dichroic mirror, 488 nm; and emission filter, 525/54 nm).

Hemocompatibility
The hemolytic activity of the new hybrids was determined using an adapted protocol based on the ASTM F 756-00 standard previously described [29]. Briefly, fresh blood was collected on heparin from healthy volunteers and diluted with PBS to a final hemoglobin concentration of~10 mg/mL. The blood was incubated with the highest concentration of the samples for 4 h at 37 • C under constant shaking. Finally, the supernatant was collected and mixed with an equal amount of Drabkin reagent (Sigma-Aldrich, Darmstadt, Germany). After 15 min, the absorbance of the samples was read at 570 nm using a plate reader. As negative and positive controls, the human red blood cells (hRBCs) in PBS and distilled water, respectively, were used. The experimental values were corrected for background dilution factors and used to calculate the percentage of hemolysis (i.e., hemolytic index), according to the equation: where A S is the corrected absorbance of the hemoglobin released in the supernatant after treatment with nanoparticles, and A T is the corrected absorbance of the total released hemoglobin.

Statistical Analysis
Unless stated otherwise, all data were expressed as the mean value ± standard deviation of three individual experiments. Statistical significance was estimated using the Student's t-test (Microsoft Excel 2010) to determine the significant differences among the experimental groups, and values of p < 0.05 were considered statistically significant.

Optical Characterization of the Developed Materials
The developed bionanosilver-based hybrid materials were optically characterized by UV-vis absorption, fluorescence emission, and FTIR spectroscopy, in order to acquire deep insights about the nanobiointeraction between components of biohybrids and also about the biohybrids' formation. Chlorophyll a (Chla) incorporated in artificial cell membranes was used as a spectral biosensor to monitor the formation of plasmonic biohybrids.
In the absorption spectra of the samples containing artificial cell membranes, the spectral signature of Chla at~669 nm was observed. Moreover, the SPR band at~431 nm, characteristic for Ag/AgClNP formation, was identified in the UV-vis absorption spectra of the silver-based materials (see Figure S1 in the Supplementary Materials).
The formation of plasmonic biohybrids was also confirmed by fluorescence emission spectra of Chla-containing samples (λ excitation = 430 nm), which underwent considerable emission quenching (see Figure S2 in the Supplementary Materials) at the interaction between the porphyrinic ring of Chla and the surface of phyto-Ag/AgClNPs. FTIR spectra allow for the identification of functional groups present in the components of the systems under investigation. The observation of the vibration spectrum of the biohybrid nanocomplexes allows evaluating the type of interaction that occurs between the Ag/AgClNPs and lecithin liposomes in the presence of chitosan or without it, as the vibrations of the atoms involved in this interaction can suffer changes in frequency and intensity (see Figure S3). These FTIR results indicate the involvement of hydroxyl and carbonyl groups (belonging to polyphenols and proteins, respectively) in the generation of biohybrids P5 and P6.
More details regarding the optical characterization of the developed materials are presented in the Supplementary Materials.

Estimation of Particle Size and Zeta Potential of the Obtained Biohybrids
The mean hydrodynamic diameters of the developed particles were estimated by DLS measurements (see Figure S4 in the Supplementary Materials). As observed, the addition of chitosan to Liposomes, Ag/AgClNPs, and Ag/AgClNPs-Liposomes resulted in a size increase. This aspect will be further confirmed by SAXS experiments and microscopic studies.
The physical stability of the suspensions of the developed particles is related to the particle electrical charge, which was quantified by zeta potential (ξ) measurements via the electrophoretic mobility of the particles in an electric field [30,31]. Great ξ magnitude is indicative of a stable system [32,33], being related to high electrical interparticle repulsion due to the surface charge, thus indicating the high stability of the suspension. Figure 2 displays the zeta potential values of the bio-based materials developed in this study. electrophoretic mobility of the particles in an electric field [30,31]. Great ξ magnitude i indicative of a stable system [32,33], being related to high electrical interparticle repulsio due to the surface charge, thus indicating the high stability of the suspension.  Chlorophyll-labeled artificial cell membranes exhibited moderate stability (ξP1 −20.17 ± 0.49 mV), and after chitosan addition, the zeta potential value increased to −8.4 ± 0.27 mV (for P2) due to the positive charge of amino functional groups in chitosan "Green" synthesized silver nanoparticles alone and embedded in biomimetic membrane registered more accentuated electronegative values (ξP3 = −31.1 ± 1.9 mV and ξP5 = −32.5 ± 1.5 mV, respectively), thus good stability. In the presence of chitosan, these value shifted to positive values: ξP4 = +17.5 ± 1.07 mV and ξP6 = +18.1 ± 0.79 mV, respectively. Th surface positivity of "green" developed nanoparticles can be attributed to their stabiliza tion with the positively charged chitosan [34].

Structural Characterization of the Biohybrid Complexes
XRD and SAXS analyses were performed to investigate the structure of the obtained materials.

X-ray Diffraction
Phase characterization and chemical composition of the liquid sediments, separated from the PBS solution by centrifugation at 4 °C, followed by evaporation at room temper ature, were performed for all samples, which included hybrid Ag/AgCl nanoparticle phytogenerated from nettles and grapes, i.e., for Samples P3-P6 ( Figure 3). All XRD spec tra demonstrate the presence of two phases: Ag and AgCl, which have a face-centered cubic (FCC) structure with a 3 space group and lattice parameters aAg = 0.40895 nm and aAgCl = 0.55487 nm, correspondingly. Moreover, it resulted from the peak intensitie that the AgCl phase substantially dominated in all the studied systems. This phenome non can be explained by two reasons. First, we demonstrate that hybrid Ag/AgCl nano particles are the result of the synthesis from biocompounds of nettle and grape aqueous ex tracts (see Section 3.1 and Supplementary Materials), as were observed in the case of th various plant extracts mediated [35,36]. Second, because of the effect of the PBS buffer when the anions of Cl − bond to Ag + , the AgCl phase becomes dominant in the compositio of Ag/AgClNPs. Two phases of NaCl and sodium hydrogen phosphate hydrate (SHPH) are remainin byproducts arising from the PBS buffer. The NaCl phase has a face-centered cubic (FCC structure with a 3 space group and a lattice parameter aNaCl = 0.5640 nm. The SHPH Sample Figure 2. Evaluation of the physical stability of the obtained bio-based materials. Chlorophyll-labeled artificial cell membranes exhibited moderate stability (ξ P1 = −20.17 ± 0.49 mV), and after chitosan addition, the zeta potential value increased to −8.45 ± 0.27 mV (for P2) due to the positive charge of amino functional groups in chitosan. "Green" synthesized silver nanoparticles alone and embedded in biomimetic membranes registered more accentuated electronegative values (ξ P3 = −31.1 ± 1.9 mV and ξ P5 = −32.57 ± 1.5 mV, respectively), thus good stability. In the presence of chitosan, these values shifted to positive values: ξ P4 = +17.5 ± 1.07 mV and ξ P6 = +18.1 ± 0.79 mV, respectively. The surface positivity of "green" developed nanoparticles can be attributed to their stabilization with the positively charged chitosan [34].

Structural Characterization of the Biohybrid Complexes
XRD and SAXS analyses were performed to investigate the structure of the obtained materials.

X-ray Diffraction
Phase characterization and chemical composition of the liquid sediments, separated from the PBS solution by centrifugation at 4 • C, followed by evaporation at room temperature, were performed for all samples, which included hybrid Ag/AgCl nanoparticles phytogenerated from nettles and grapes, i.e., for Samples P3-P6 ( Figure 3). All XRD spectra demonstrate the presence of two phases: Ag and AgCl, which have a face-centered cubic (FCC) structure with a Fm3m space group and lattice parameters a Ag = 0.40895 nm and a AgCl = 0.55487 nm, correspondingly. Moreover, it resulted from the peak intensities that the AgCl phase substantially dominated in all the studied systems. This phenomenon can be explained by two reasons. First, we demonstrate that hybrid Ag/AgCl nanoparticles are the result of the synthesis from biocompounds of nettle and grape aqueous extracts (see Section 3.1 and Supplementary Materials), as were observed in the case of the various plant extracts mediated [35,36]. Second, because of the effect of the PBS buffer, when the anions of Cl − bond to Ag + , the AgCl phase becomes dominant in the composition of Ag/AgClNPs. Two phases of NaCl and sodium hydrogen phosphate hydrate (SHPH) are remaining byproducts arising from the PBS buffer. The NaCl phase has a face-centered cubic (FCC) structure with a Fm3m space group and a lattice parameter a NaCl = 0.5640 nm. The SHPH phase with chemical formula Na 2 HPO 3 (H 2 O) 5 has an orthorhombic structure (space group Pmn2 1 ) with lattice parameters a = 0.7170 nm, b = 0.6360 nm, and c = 0.9070 nm [37]. The average crystallite sizes of the nanoparticles (D XRD ) for each phase, estimated using the Scherrer equation (Equation (1)), are collected in Table 2.
phase with chemical formula Na2HPO3(H2O)5 has an orthorhombic structure (space group Pmn21) with lattice parameters a = 0.7170 nm, b = 0.6360 nm, and c = 0.9070 nm [37]. The average crystallite sizes of the nanoparticles (DXRD) for each phase, estimated using the Scherrer equation (Equation (1)), are collected in Table 2.

SAXS Results
Small-angle X-ray scattering was used to study the structural changes of the Ag/AgCl nanoparticles in the biohybrid complexes P3-P6 in excess of PBS medium at the nanoscale level.
The proposed model (Guinier-Porod) allows for the determination of the size and dimensionality of the objects (see Supplementary Materials). Scattering curves for P3, P4, and P5 are quite similar [38]. The SAXS experimental data for the initial components and

SAXS Results
Small-angle X-ray scattering was used to study the structural changes of the Ag/AgCl nanoparticles in the biohybrid complexes P3-P6 in excess of PBS medium at the nanoscale level.
The proposed model (Guinier-Porod) allows for the determination of the size and dimensionality of the objects (see Supplementary Materials). Scattering curves for P3, P4, and P5 are quite similar [38]. The SAXS experimental data for the initial components and their complexes are shown in Figure 4. The obtained parameters from the fitting procedure on the experimental SAXS data are presented in Table 3.  Best fits are presented in Figure 4 as lines. The presence of two structural levels is clearly seen from the SAXS curves. The scattering objects were tentatively divided into two parts: smaller nanoparticles with Rg1 ranging from 10.1 nm up to 15.7 nm and larger nanoparticles with Rg2 ranging from 33.7 nm up to 43.4 nm. Based on the dimensionality value(s), we can assume a spherical shape of NPs. Then, the average diameter can be calculated as DSAXS = 2(5/3) 1/2 Rg. The obtained values are presented in Table 3.   Table 3. Structural parameters derived from the analysis of SAXS data and the calculated diameter (D SAXS = 2(5/3) 1/2 R g ) of the Ag and Ag/AgCl nanoparticles for silver-based samples (P3-P6). Best fits are presented in Figure 4 as lines. The presence of two structural levels is clearly seen from the SAXS curves. The scattering objects were tentatively divided into two parts: smaller nanoparticles with R g1 ranging from 10.1 nm up to 15.7 nm and larger nanoparticles with R g2 ranging from 33.7 nm up to 43.4 nm. Based on the dimensionality value(s), we can assume a spherical shape of NPs. Then, the average diameter can be calculated as D SAXS = 2(5/3) 1/2 R g . The obtained values are presented in Table 3.

Silver-Based
SAXS and XRD results both confirm the presence of two types of nanoparticles in the system: AgNPs and hybrid Ag/AgClNPs. The findings achieved through XRD and SAXS analyses support the results obtained by UV-vis absorption spectroscopy. Thus, the mixture with CTS (Sample P4) increased to a larger diameter by 5 nm, while in the sample with liposomes (Sample P5), we observed an increase by 25 nm. Interestingly, the scattering curve for Sample P6 slightly differs from other complexes with Ag/AgClNPs. The size of the small nanoparticles is identical to the values determined for the previously discussed samples, while the larger nanoparticles are much smaller than observed for Samples P3-P5. Note that the small NPs containing Ag crystallites have a diffusive interface [39], resulting in higher anisotropy objects and thus higher values of the dimensionality parameter. For larger Ag/AgClNPs, the power-law exponent implies that scattering occurs on the mass fractals with a fractal dimension of~3 [39][40][41][42].

Morphological Characterization of the Developed Bio-Based Materials
The surface characteristics of the biohybrids were studied using AFM and SEM methods.

AFM Analysis of the Developed Materials
AFM topology of the hybrid Ag/AgClNPs is shown in Figure 5 (left). The NPs have a spherical shape, which is in good agreement with the results obtained from the approximation of the SAXS curves (see Figure 4). The average size of Ag/AgClNPs is 48.2 ± 9.5 nm. Silver/silver chloride nanoparticles in the presence of chitosan are involved in the polymer network, as is clearly seen in Figure 5 (right).  Ag/AgClNPs coated with chitosan have an average size of 56.9 ± 19.5 nm. The size distribution includes aggregates ranging in size from 75 to 100 nm. Biohybrid Complex I consists of NPs with a chitosan shell, indicated by the following items: (1) an increase in NP size; (2) an increase in surface roughness (R a_P3 = 0.5 nm, R a_P4 = 0.7 nm, R q_P3 = 0.57 nm, and R q_P4 = 0.9 nm); and (3) the appearance of a rough surface of Ag/AgClNPs in the presence of CTS compared to the smooth surface of Ag/AgClNPs without CTS, as can be clearly seen from the height analysis and magnified 3D images for P3 and P4 systems ( Figure 5, bottom figures).
Low height is, according to AFM, a flattening effect that occurs during the adsorption of the nanoparticles on mica and their drying. More details regarding the sonication time effect on liposome formation are given in Figure S5 in the Supplementary Materials.
AFM images for biohybrid complexes II (P5) and III (P6) are demonstrated in Figure 6. In both cases, the presence of Ag/AgClNPs on the surface of the liposomes was detected (green crops from scan images). Obviously, the morphology of the liposomes is changed: they have an ellipsoidal shape with an apparent width (W, in its short axis) of ∼341 nm and length (L, in its long axis) of ∼516 nm for the P5 system, and W ≈ 480 nm and L ≈ 660 nm for the P6 system, while most liposomes in the AFM images of the P1 and P2 systems appear regularly spherical and not deformed (see Figure S5 in the Supplementary Materials). The sizes of hybrid Ag/AgClNPs associated with liposomes (highlighted by circles in green crops) are 64-77 nm and 97-172 nm for biohybrids P5 and P6, respectively.
The average size of Biohybrid P5 obtained from the AFM image (Figure 6a) is 72.6 ± 18.2 nm, and this value is in good agreement with 76.3 nm obtained from SAXS (see Supplementary Materials).
A close examination of the area highlighted in orange in Figure 6b indicates the presence of "free" silver/silver chloride nanoparticles with an almost spherical shape and sizes between 42 and 78 nm, which is consistent with the values of 39.5 and 60.9 nm obtained from the SAXS method. The central NP has a dimension of 112 nm. Such larger nanoparticle sizes, from which SAXS scattering was not detected due to method limitations, are present over the entire studied area (Figure 6b, top image), and we assume they are nanoparticle aggregates. Figure 7 presents the SEM images of Samples P1 up to P6 and a magnified area of 3 × 3 µm 2 . As one can observe, the samples are not identical in their morphologies. They present various structures with different shapes and sizes. For instance, Sample P1 shows individual spherical shape structures of lipid vesicles, whereas Sample P2 exhibits chainlike structures due to the presence of chitosan, including spherical structures in the mesh of the network. The silver nanoparticles without (Sample P3) and with (Sample P4) chitosan are spread all over the silicon plate surface. However, Sample P5 shows micrometric structures, and Sample P6 shows nano-and micrometric entities. This behavior can be explained by the diversity in the synthesis procedure of the samples, as explained in Table 1. As observed, the addition of chitosan resulted in increasing size of the samples, in good agreement with UV-vis absorption spectra, DLS results, SAXS data, and AFM analysis.

SEM Analysis of the Developed Bio-Based Materials
The average size of Biohybrid P5 obtained from the AFM image (Figure 6a) is 72.6 ± 18.2 nm, and this value is in good agreement with 76.3 nm obtained from SAXS (see Supplementary Materials).
A close examination of the area highlighted in orange in Figure 6b indicates the presence of "free" silver/silver chloride nanoparticles with an almost spherical shape and sizes between 42 and 78 nm, which is consistent with the values of 39.5 and 60.9 nm obtained from the SAXS method. The central NP has a dimension of 112 nm. Such larger nanoparticle sizes, from which SAXS scattering was not detected due to method limitations, are present over the entire studied area (Figure 6b, top image), and we assume they are nanoparticle aggregates. Figure 7 presents the SEM images of Samples P1 up to P6 and a magnified area of 3 × 3 µm 2 . As one can observe, the samples are not identical in their morphologies. They present various structures with different shapes and sizes. For instance, Sample P1 shows individual spherical shape structures of lipid vesicles, whereas Sample P2 exhibits chainlike structures due to the presence of chitosan, including spherical structures in the mesh of the network. The silver nanoparticles without (Sample P3) and with (Sample P4) chitosan are spread all over the silicon plate surface. However, Sample P5 shows micrometric structures, and Sample P6 shows nano-and micrometric entities. This behavior can be explained by the diversity in the synthesis procedure of the samples, as explained in Table  1. As observed, the addition of chitosan resulted in increasing size of the samples, in good agreement with UV-vis absorption spectra, DLS results, SAXS data, and AFM analysis.

Mechanism of Biohybrid Formation
Summarizing our optical, structural, and morphological investigations, as well as the stability study of the biohybrid complexes and their components, a mechanism of Ag/AgClNP fabrication and biohybrid formation, can be discussed.
Biohybrid Complex I (Ag/AgClNPs-CTS) with the proposed interaction model between the chitosan matrix and silver/silver chloride nanoparticles is shown schematically in Figure 8. The silver ions' interaction takes place through the amino and hydroxyl groups of chitosan [43]. Moreover, it could be assumed that the formation of the chitosan-capped Ag/AgClNPs was confirmed by zeta potential measurements and by SAXS, SEM, and AFM studies. tween the chitosan matrix and silver/silver chloride nanoparticles is shown schematic in Figure 8. The silver ions' interaction takes place through the amino and hydro groups of chitosan [43]. Moreover, it could be assumed that the formation of the chitos capped Ag/AgClNPs was confirmed by zeta potential measurements and by SAXS, SE and AFM studies. Biohybrid II (Ag/AgClNPs-Lip) is a multilamellar vesicle (MLVs) with a surf coated with nanoparticles ( Figure 8B). This output was obtained from a mixture of soyb lecithin liposomes and silver/silver chloride nanoparticles in PBS after sonication of Biohybrid II (Ag/AgClNPs-Lip) is a multilamellar vesicle (MLVs) with a surface coated with nanoparticles ( Figure 8B). This output was obtained from a mixture of soybean lecithin liposomes and silver/silver chloride nanoparticles in PBS after sonication of the suspension for 5 min. Such a short time of treatment of the suspension with ultrasound does not lead to the formation of unilamellar vesicles (ULVs) and excludes with a high degree of probability the creation of other possible systems: (1) liposomes with bilayerembedded nanoparticles, (2) liposomes with core-encapsulated nanoparticles, and (3) lipid-bilayer-coated nanoparticles. The obtained complex is a very stable system, as indicated by the zeta potential value of −33 mV. In addition, this value is very close to −31.7 mV for Ag/AgClNPs, and this result indicates the adhesion of nanoparticles on the liposome surface. At the same time, the interaction of Ag/AgClNPs with liposomes causes a change in liposome morphology. The ellipsoidal shape was observed by the AFM method, while the pure soybean lecithin liposomes were almost spherical, as clearly seen on the microscopic images ( Figure S5a-c in the Supplementary Materials and Figure 6a). A similar effect was detected for Biohybrid III (Ag/AgClNPs-Lip-CTS): liposomes surrounded by chitosan have a spherical shape, and liposome-nanoparticles systems involved in the 3D chitosan network have an ellipsoidal shape ( Figure S5d,e in the Supplementary Materials and Figure 6b). Even though this complex is less stable (ξ = +18.4 mV) than previously described, it has high antioxidant activity and antibacterial effectiveness, as will be further presented in Section 3.6.

Evaluation of Biological Activities of the Developed Bio-Based Materials
The in vitro bioactivities of materials phytogenerated from an aqueous extract of a mixture of nettle and grapes were tested by assessing: the antioxidant activity, the antibacterial properties against S. aureus and E. coli, the cytotoxicity, the antiproliferative activity, and the hemocompatibility. A therapeutic index was also calculated for each sample.
The biological performances of the developed materials were closely related to their zeta potential values, size, morphology, and structure.
The samples showed good antioxidant activity, ranging from 62 to 75% (in vitro tested through the chemiluminescence method; see Figure 9). change in liposome morphology. The ellipsoidal shape was observed by the AFM while the pure soybean lecithin liposomes were almost spherical, as clearly seen microscopic images ( Figure S5a-c in the Supplementary Materials and Figure 6a) ilar effect was detected for Biohybrid III (Ag/AgClNPs-Lip-CTS): liposomes surr by chitosan have a spherical shape, and liposome-nanoparticles systems involve 3D chitosan network have an ellipsoidal shape ( Figure S5d,e in the Supplementar rials and Figure 6b). Even though this complex is less stable (ξ = +18.4 mV) than pre described, it has high antioxidant activity and antibacterial effectiveness, as will be presented in Section 3.6.

Evaluation of Biological Activities of the Developed Bio-Based Materials
The in vitro bioactivities of materials phytogenerated from an aqueous ext mixture of nettle and grapes were tested by assessing: the antioxidant activity, t bacterial properties against S. aureus and E. coli, the cytotoxicity, the antiprolifer tivity, and the hemocompatibility. A therapeutic index was also calculated for ea ple.
The biological performances of the developed materials were closely related zeta potential values, size, morphology, and structure.
The samples showed good antioxidant activity, ranging from 62 to 75% (in vit through the chemiluminescence method; see Figure 9).
The good effectiveness of Ag/AgClNPs-based materials in the scavenging ac reactive oxygen species (ROS) is explained by: (i) their composition (especially t ence of "green" Ag/AgClNPs carrying antioxidant molecules such as polypheno rophyll, etc., arising from vegetal extracts) and (ii) their nanosized dimensions (w fer more reaction centers for ROS scavenging) [27]. Antibacterial effectiveness of the developed biohybrids was tested against S coccus aureus ATTC 2592 (as a representative Gram (+) bacteria) and Escherichia co 8738 (as a representative Gram (-) bacteria) studied by the agar well diffusion met Figure 10). The good effectiveness of Ag/AgClNPs-based materials in the scavenging activity of reactive oxygen species (ROS) is explained by: (i) their composition (especially the presence of "green" Ag/AgClNPs carrying antioxidant molecules such as polyphenols, chlorophyll, etc., arising from vegetal extracts) and (ii) their nanosized dimensions (which offer more reaction centers for ROS scavenging) [27].
Antibacterial effectiveness of the developed biohybrids was tested against Staphylococcus aureus ATTC 2592 (as a representative Gram (+) bacteria) and Escherichia coli ATCC 8738 (as a representative Gram (-) bacteria) studied by the agar well diffusion method (see Figure 10). ous health problems [44].
Our "green" obtained Ag/AgClNPs are more efficient against the two pathogens S. aureus and E. coli (IGZ S. aureus = 20 mm; IGZ E. coli = 13 mm) as compared to the AgClNPs prepared by Trinh et al. [45], who obtained IGZ values less than 11 mm for both strains. Kashyap et al. [20] prepared Ag/AgCl particles showing a zone of inhibition of 7.5 mm against E. Coli. Moreover, AgClNPs synthesized by Kota et al. [21] proved to be less potent against S. aureus (IGZ S. aureus = 18.5 mm) as compared to our silver nanoparticles. The biohybrids containing "green" Ag/AgClNPs and Chla-Liposomes (Biohybrid II) exhibited high antibacterial properties against Staphylococcus aureus ATTC 2592 (IGZ = 25 mm) and Escherichia coli ATCC 8738 (IGZ = 40 mm) (see Sample P5 in Figure 10), as compared to Biohybrid I, which showed an IGZ value of 20 mm against E. coli and 22 mm against S. aureus (see Sample P4 in Figure 10).
These developed materials showed different behavior against two bacterial strains due to the differences in the bacterial cell wall structures. Gram (+) bacteria possess a thick peptidoglycan layer and no outer lipid membrane, while Gram (-) bacteria have an outer lipid membrane with pores and a unique periplasmic space with a thin peptidoglycan layer [46].
Direct contact of our developed materials with the bacterial cells resulting in perturbation/deterioration of cell walls and membranes leading to cell death is the most plausible antibacterial mechanism [47][48][49]. The need for creating new antibacterial systems is an important research area in the medical field. Staphylococcus aureus and Escherichia coli are the most important human pathogens associated with nosocomial and community-acquired infections, causing serious health problems [44].
Our "green" obtained Ag/AgClNPs are more efficient against the two pathogens S. aureus and E. coli (IGZ S. aureus = 20 mm; IGZ E. coli = 13 mm) as compared to the AgClNPs prepared by Trinh et al. [45], who obtained IGZ values less than 11 mm for both strains. Kashyap et al. [20] prepared Ag/AgCl particles showing a zone of inhibition of 7.5 mm against E. Coli. Moreover, AgClNPs synthesized by Kota et al. [21] proved to be less potent against S. aureus (IGZ S. aureus = 18.5 mm) as compared to our silver nanoparticles.
These developed materials showed different behavior against two bacterial strains due to the differences in the bacterial cell wall structures. Gram (+) bacteria possess a thick peptidoglycan layer and no outer lipid membrane, while Gram (-) bacteria have an outer lipid membrane with pores and a unique periplasmic space with a thin peptidoglycan layer [46]. Direct contact of our developed materials with the bacterial cells resulting in perturbation/deterioration of cell walls and membranes leading to cell death is the most plausible antibacterial mechanism [47][48][49].
Cell viability results are reported in Figure 11 for all three cell lines investigated, highlighting the dependence of cell viability on the silver content and the type of cell line. Low doses of AgNPs had less cytotoxicity on the growth of normal cell lines (BJ cells), but enhanced cytotoxicity was observed with increasing doses. The results obtained are in correlation with those reported in the literature [50,51]. It was found that at concentrations less than 25.5 µM, the samples do not show a toxic effect, the cell viability being higher than 80% in the case of BJ cells. Chitosan addition to the AgNPs did not improve the efficiency of the NPs but only increased the overall concentration where the effect was observed. A better efficiency was observed for the samples prepared with the liposomes. Thus, the most efficient proved to be the NPs prepared with liposomes, P5 and P6, especially Sample P6, which, over the entire range, tested displayed less toxicity to normal cells and increased toxicity to cancer cells. Cell viability results are reported in Figure 11 for all three cell lines investigated, highlighting the dependence of cell viability on the silver content and the type of cell line. Low doses of AgNPs had less cytotoxicity on the growth of normal cell lines (BJ cells), but enhanced cytotoxicity was observed with increasing doses. The results obtained are in correlation with those reported in the literature [50,51]. It was found that at concentrations less than 25.5 µM, the samples do not show a toxic effect, the cell viability being higher than 80% in the case of BJ cells. Chitosan addition to the AgNPs did not improve the efficiency of the NPs but only increased the overall concentration where the effect was observed. A better efficiency was observed for the samples prepared with the liposomes. Thus, the most efficient proved to be the NPs prepared with liposomes, P5 and P6, especially Sample P6, which, over the entire range, tested displayed less toxicity to normal cells and increased toxicity to cancer cells. The values of IC50 and the therapeutic index (TI) are reported in Table 4. IC50 values were used further to calculate the TI, which is an indicator of the treatment efficiency against cancer cells. A value higher than one of TI indicates that the anticancer activity is higher compared with the cytotoxic activity of the samples investigated against the normal cells (BJ cells) [28].  Table 4. IC 50 values were used further to calculate the TI, which is an indicator of the treatment efficiency against cancer cells. A value higher than one of TI indicates that the anticancer activity is higher compared with the cytotoxic activity of the samples investigated against the normal cells (BJ cells) [28]. From Table 4, one can see that Samples P3, P5, and P6 are more efficient against HepG2 cells, while P5 and P6 against HT-29 cells. The results indicated that Samples P3 and P4, which have in their composition only Ag and Ag and chitosan, respectively, are more toxic for normal cells as compared to cancerous cells. However, after the addition of lipids to the samples (P5 and P6), their efficacy increased, mainly by observing an increase in the toxicity against cancer cells.
Further, we investigated the effect induced by the highest concentration of the samples tested before against the red blood cells. At 102.2 µM, for each sample, the hemolysis percentage of new silver-based hybrids ( Figure 12) is far below 5% [29], meaning that these samples are slightly hemolytic, but they will not be harmful when found in the bloodstream at smaller concentrations.   Table 4, one can see that Samples P3, P5, and P6 are more efficient against HepG2 cells, while P5 and P6 against HT-29 cells. The results indicated that Samples P3 and P4, which have in their composition only Ag and Ag and chitosan, respectively, are more toxic for normal cells as compared to cancerous cells. However, after the addition of lipids to the samples (P5 and P6), their efficacy increased, mainly by observing an increase in the toxicity against cancer cells.
Further, we investigated the effect induced by the highest concentration of the samples tested before against the red blood cells. At 102.2 µM, for each sample, the hemolysis percentage of new silver-based hybrids ( Figure 12) is far below 5% [29], meaning that these samples are slightly hemolytic, but they will not be harmful when found in the bloodstream at smaller concentrations.       The control BJ cells normally present an elongated shape and when treated with the smallest concentration of the sample, it could be observed that the morphology of these cells was not affected ( Figure 13). However, at 51.1 µM silver content, the cells' morphology was drastically affected: the cells' branches were reduced, as well as the cell body. The results are in correlation with those reported for cell viability, where at 51.1 µM, the viability decreased by around 30-40% for all the samples investigated. Figure 14 presents the morphological changes of HT-29 cells induced by different treatments. Control HT-29 cells grow in clusters as observed in Figure 14A. When treated with 6.4 µM, we can observe that the morphology of the cells was nonsignificantly affected. At 51.1 µM, the cells' morphology is affected as well as the reduction of the number of cells.
In Figure 15 are presented the results for HepG2 cells. Control HepG2 cells grow in clusters, as observed in Figure 15A. When treated with 6.4 µM, we can observe that the morphology of the cells is not affected so much. However, at 51.1 µM, the number of cells is reduced. For both HT-29 and HepG2 cells, the results reported are in good concordance with the results reported for cell viability.
To summarize, the results obtained regarding the biological activity of the prepared materials are encouraging, taking into account that good bioperformances were obtained at a lower silver content compared to the data previously reported by our research group [10,27].

Conclusions
Vegetal wastes of grapes and nettle leaves were used to generate biohybrid entities by using the Green Chemistry principles.
The natural porphyrin chlorophyll a, inserted in biomimetic membranes, acted as a spectral sensor to monitor the generation of the biohybrids. The biointeraction between bionanometals and artificial cell membranes was detected by Chla at the nano level, through changes in its spectral fingerprints.
The optical, structural, and morphological investigations correlated well, and the mechanism of Ag/AgClNP fabrication and biohybrid formation was discussed.
Microscopical investigations by AFM and SEM images gave information about the (quasi)spherical morphology and nanoscaled size of the samples.
XRD and SAXS investigations revealed the structural changes of the Ag/AgCl nanoparticles in the biohybrid complexes, highlighting the copresence of AgNPs and hybrid Ag/AgClNPs in the obtained silver-based systems. Particular attention was paid to the study of Biohybrid III (Ag/AgClNPs-Liposomes-CTS) because during the formation of biohybrid complexes, namely liposomes NPs, there is a high probability that small nanoparticles, such as AgNPs, may pass through the cell membranes, thereby affecting their functionality. However, in our case, it can be assumed that silver chloride nanoparticles (AgClNPs) or hybrid Ag/AgClNPs, being large in size, do not disturb the integrity of the membrane and accumulate on their outer leaflet, shown by the mechanism of biohybrid formation proposed by us.
Coincorporation of Chla-labeled mimetic biomembranes, Ag/AgClNPs and chitosan, resulted in significant bioperformances. The obtained silver-based biohybrids showed good antioxidant properties by scavenging 71% of reactive oxygen species and also presented high antimicrobial activity against Escherichia coli (IGZ = 45 mm) and Staphylococcus aureus (IGZ = 30 mm). The silver/biomimetic membrane biohybrids with and without chitosan were hemocompatible and presented efficiency against HepG2 and HT-29 cancer cells. The therapeutic index of Ag/AgClNPs-Liposomes-CTS samples supports the antitumor effect; these biohybrids exhibited a TI value of 1.30 for HT-29 cancer cells and 1.77 for HepG2 cancer cells, highlighting their antitumor effect against two types of cell lines.
These results demonstrate that silver-containing hybrid entities could be used as building blocks to design new materials with many bioapplications, especially in the treatment of liver and colorectal cancer.

Data Availability Statement:
The data is included in the main text and/or the supplementary materials.

Conflicts of Interest:
The authors declare no conflict of interest.